|Year : 2010 | Volume
| Issue : 2 | Page : 65-70
|In vitro comparison of the radiopacity of cavity lining materials with human dental structures
Fernanda CP Pires de Souza1, Luiz C Pardini2, Diogo R Cruvinel1, Hisham M Hamida1, Lucas FR Garcia1
1 Department of Dental Materials and Prosthodontics, Ribeirao Preto School of Dentistry, University of São Paulo, Ribeirao Preto, SP, Brazil
2 Department of Morphology, Stomatology, and Physiology, Ribeirao Preto School of Dentistry, University of São Paulo, Ribeirao Preto, SP, Brazil
Click here for correspondence address and email
|Date of Submission||17-Feb-2010|
|Date of Decision||17-Mar-2010|
|Date of Acceptance||08-Apr-2010|
|Date of Web Publication||23-Jul-2010|
| Abstract|| |
Aim: To compare the optical densities (OD) of calcium hydroxide (CH) and glass ionomer cement with the same thicknesses of the dental structures.
Materials and Methods: Eighteen specimens of each material, with thicknesses of 0.5, 1.0, 1.5, 2.0, 2.5, and 3.0 mm were made in a Teflon matrix. To compare the radiopacity of the materials with the dental structures, dental cuts of the first molars, increasing in thickness from 0.5 to 3.0 mm, were obtained. To standardize the radiographs, a transparent acrylic matrix (Standardizing Device) was developed and used. Thirty radiographs were taken, five for each tested material.
Results: Statistical analysis (Two-way ANOVA - Bonferroni, P < 0.05) demonstrated that when the materials were compared, there was statistically significant difference between the ODs, only for the thickness of 1.0 mm (P < 0.05).
Conclusion: The thickness of the material contributed to its radiopacity, and these materials had to be used in a thickness between 1.5 and 2.0 mm.
Keywords: Calcium hydroxide; dentin; enamel; glass ionomer cement; radiopacity
|How to cite this article:|
Pires de Souza FC, Pardini LC, Cruvinel DR, Hamida HM, Garcia LF. In vitro comparison of the radiopacity of cavity lining materials with human dental structures. J Conserv Dent 2010;13:65-70
|How to cite this URL:|
Pires de Souza FC, Pardini LC, Cruvinel DR, Hamida HM, Garcia LF. In vitro comparison of the radiopacity of cavity lining materials with human dental structures. J Conserv Dent [serial online] 2010 [cited 2020 Jul 14];13:65-70. Available from: http://www.jcd.org.in/text.asp?2010/13/2/65/66713
| Introduction|| |
Ideally, the materials used for dentin-pulp complex protection should present, among other properties, sufficient radiopacity, to be distinguished from the adjacent anatomical structures, such as, dentin and enamel. ,
At present two materials are widely disseminated and used for this purpose: glass ionomer cements (GIC) and calcium hydroxide (CH); the latter has the properties of stimulating the formation of sclerotic and reparative dentin  and protects the pulp against thermal electric stimuli  and antibacterial action. , GIC also has several favorable properties and among them, the fluoride release that diminishes the incidence of secondary caries lesions, coefficient of thermal expansion similar to that of the tooth, pulp biocompatibility, and reduction in microleakage are pointed out. ,,
Ideally, the materials must present sufficient radiopacity to enable them to be differentiated from the adjacent anatomic structures, , facilitating the evaluation of restorations and enabling the detection of secondary caries, ,,,,, because radiolucent materials may conceal the early diagnosis of some lesions. 
Several factors may affect the radiopacity of dental materials, but the composition seems to be the most important factor.  The higher the atomic number (Z) of the metal chemical elements present in the composition of the materials, higher is their capacity to absorb X-rays.  In addition, the material thickness, , angulation of the X-ray beam, methodology used for evaluation,  type of X-ray film, and radiographic processing can also have an influence. 
The degree of radiopacity required for an ideal clinical performance may vary according to the class of the material.  Some authors consider that the radiopacity of the material must be equal or higher than the radiopacity of dentin, to guarantee that the material is not confounded with carious dentin.  Others consider that the restorative material needs a slightly higher degree of radiopacity than enamel. ,,,, Nevertheless, several studies have assessed radiopacity from a 2 mm-increment graduated aluminum step-wedge, varying from 2 to 16 mm in thickness. ,,,
The GIC is radiolucent because it is composed of light elements. , To increase its visibility in this sense, barium or zinc oxide glass is incorporated into it. In some products, the calcium (Z = 20) present in the composition has been replaced by strontium, which has a chemically similar behavior (Z = 38), and gives the material a greater capacity to absorb X-rays. 
However, CH cements are presented in the form of two components that set when they are mixed. The accelerator paste is composed of calcium hydroxide, zinc oxide, zinc stearate, and a vehicle. The base paste is composed of glycolic salicylate - the basic ingredient required for the setting reaction to occur - in addition to titanium dioxide, calcium sulfate, and calcium tungsten, which are inert particles serving as radiopacifiers. 
The aim of this study is to compare the optical densities of different thicknesses of pulp protecting materials (calcium hydroxide and glass ionomer cements) having the same thickness of dental structures (enamel and dentin). The hypothesis of this study is that the thicker the layer of lining material, the more radiopaque is its radiographic image. Another hypothesis that has been tested is that lining materials have different optical densities from those of the dental structures, irrespective of their thickness, allowing a differential diagnosis of its radiographic image.
| Materials and Methods|| |
To conduct this study, the materials listed in [Table 1] were selected.
All the geometrical factors that might interfere in the formation of the radiographic image were standardized by creating a transparent acrylic matrix called the Standardizing Device, measuring 8 ΄ 7 cm. These measurements corresponded to the width and length of an occlusal radiographic film, which was adapted to the bottom part of the device, fixed on lateral channels [Figure 1]. The upper part of the device was composed of steps that gradually increased in thickness every 0.5 mm up to the thickness of 3.0 mm. Therefore, the first step was 0.5 mm thick, the second 1.0 mm, and so on, up to the last step of 3.0 mm thickness, which was a total of six steps. On each step, three circular orifices measuring 5 mm in diameter were opened, to place the material to be radiographed, totaling to 18 orifices.
An opening was made in the center of the thickness Standardizing Device, suitable for adapting the aluminum scale (penetrometer), measuring 10 Χ 32 mm, and scaled in eight steps, with incremental thicknesses of 2.0, 4.0, 6.0, 8.0, 10.0, 12.0, 14.0, and 16.0 mm, according to the recommendations of Manson-Hing and Bloxom.  The purpose of this penetrometer was to simulate, by means of shade nuances produced after exposure and processing of the radiographs, the densities of the structures of the oral cavity in comparison to the hard and soft tissues, for laboratorial analyses of the quality of the radiographic images, to show the homogeneity of the procedures, and to detect possible variations during the procedures of the radiographic techniques and processing.
To certify that the acrylic material of the thickness Standardizing Device would not interfere with the radiographic image of the materials, an initial radiographic image was taken with an occlusal film (Insight, Kodak, New York, NY, USA) and the penetrometer only.
After receiving approval from the Research Ethics Committee of the Dentistry School of Ribeirγo Preto - University of Sγo Paulo (Process N 2005.1.1374.58.0), the study was conducted to compare the radiopacity of the material with the dental structures (enamel and dentin). Dental cuts increasing in thickness from 0.5 to 3.0 mm were obtained from six healthy adult teeth (first molar), with one cut being taken from each tooth. These slices were acquired by sectioning the tooth in the mesio-distal direction with a diamond disk (Buehler, Lake Bluff, IL, USA) cut in a microtome (MTI Corporation, Richmond, CA, USA), in order to obtain regular dental slices with enamel and dentin, with thicknesses of 0.5, 1.0, 1.5, 2.0, 2.5, and 3.0 mm [Figure 2]. The slices were stored in artificial saliva in an oven at a temperature of 37.5ΊC before performing the experiment.
To regularize the two sides of these cuts and in order to assure that they presented the recommended thickness for the experiment, the dental cuts were submitted to polishing, using 800 grain water abrasive papers (Norton Abrasivos Brasil, Sγo Paulo, SP, Brazil), in a manual polishing machine. The thickness was strictly controlled with the aid of a digital pachymeter (Digimess, Sγo Paulo, SP, Brazil).
The test specimens of each material were obtained at thicknesses of 0.5, 1.0, 1.5, 2.0, 2.5, and 3.0 mm by manipulating the materials strictly in accordance with the manufacturers' recommendations. Thus, after manipulation, the materials were immediately placed in a Teflon matrix formed by two parts fitted together: one external and the other an internal portion, in the form of a plunger, with an internal diameter of 5 mm. Accompanying the matrix, the spacers were placed according to the thickness of the test specimen that was to be obtained. These spacers were fitted into the plunger between the top and bottom portion of the matrix, so that the external part of the matrix would provide the adequate thickness of the test specimen [Figure 3]. After the material had set, the spacer was removed by lowering the matrix plunger, which released the test specimen.
Eighteen test specimens of each studied material were made, three of each thickness. After obtaining the test specimens, they were fitted in the orifices of the matrix and radiographed. For this procedure, occlusal radiographic films (Insight, Kodak, Nova York, NY, EUA) sensitivity group 'E' (REF 1169143, Lot 4107790) and an X-ray appliance (Dabi Atlante, Ribeirγo Preto, SP, Brazil) with a central opening, 11 mm in diameter, were used. Pilot tests were conducted to determine the exposure time of 0.5 seconds, which was defined as that which presented an optical density of 1 (+) in the radiographic image of 10 mm step wedge thickness. In addition to the materials tested, the dental disks with thicknesses according to the step height were placed next to the orifices on each step [Figure 4].
The locator cylinder was adjusted perpendicular to the Standardizing Device, at a focus-film distance of 20 cm and set for 70 kVp, with exposure time of 0.5 seconds. After taking the radiographs, the films were submitted to a manual developing process, following the manufacturer's recommendations with regard to the time / temperature processing method.
Thirty radiographs were taken, five for each material tested. The optical density value (OD) readouts were performed with the aid of a photodensitometer (Gafchromic, Victoreen, Moedling, Austria) with the collimated light beam of 1 mm in diameter. Three OD readouts were made for each step of the penetrometer, for each sample and dental cut (enamel and dentin) per thickness.
After the readouts and after verifying the normality of the sample (Kolmogorov-Smirnov test), the means and respective standard deviations of the optical density values of each tested material were calculated, which were submitted for statistical analysis (two-way ANOVA - Bonferroni, P < 0.05).
| Results|| |
Comparison of the OD means of the materials and dental structures may be seen in [Table 2] and [Figure 5]. Analyses of the data allowed one to verify that as the thickness increased, the OD diminished; that is, the image became gradually more radiopaque. A mean variation in OD between 1.25 and 2.33 was shown for the enamel, and from 1.45 to 2.36 for dentin. This indicated that dentin showed more radiolucence than enamel at all thicknesses; however, there was a statistically significant difference (P < 0.05) only from 2.0 mm.
The mean OD of CH ranged from 1.15 to 2.14. At all thicknesses, its OD was lower than that of the dental structures, differing statistically from dentin at all thicknesses, and from enamel at the thicknesses of 0.5, 1.0, and 2.5 mm (p < 0.05). CIG also showed an OD lower than that of the dental structures, with the exception of thickness 2.0 mm, which presented a higher OD than the same enamel thickness, however, with no statistically significant difference (P > 0.05).
When comparing the materials between them, it was verified that there was a statistically significant difference (P < 0.05) between the OD only for the thickness of 1.0 mm. For the other thicknesses, there was no statistically significant difference (P > 0.05).
| Discussion|| |
Radiopacity is an important scientific property of dental materials and can be simply defined as the inverse of the optical density of a radiographic image. Optical density provides a measure of how dark the developed film can appear, as perceived by the human eye.  It consists of two inherent values: fog and base density. In the absence of any exposure of the undeveloped film to X-rays, a developed film will nevertheless show some absorption of light. This is called fog. Under normal conditions of measurement, the optical density of the processed emulsion of the film will be indistinguishable from the fog, due to light absorption and scattering components. However, the radiographic film for dental use is usually sold with a blue- or gray-tinted base, to improve the image visualization by the human eye and this is known as base density. 
The base and fog value is the inherent optical transmission density (lowest density) of a film base plus the non-image density contributed by the developed emulsion.  Optical density is a logarithmic measure of the ratio of transmitted to incident light through the film image, and depends not only on the inherent X-ray absorption properties of the materials, but also on the characteristics of the film, its exposure parameters, and processing conditions.  In this study, all these variables were standardized. Thus, any difference in optical density and hence in radiopacity was due to the different properties of materials.
The studied materials were shown to have radiopacifiers in their composition appropriate to the formation of their radiographic images. , One of the hypotheses tested showed that the thicker the layer of lining material, the more radiopaque it had in its radiographic image. The analyses of the results allowed one to agree with the hypotheses tested only for GIC. However, for CH, there was no statistically significant difference in the optical density from the thickness of 2.5 mm in comparison with the thickness of 3.0 mm (P > 0.05). This demonstrated a limitation in the penetration power of the X-ray into CH; that is, irrespective of the increase in thickness of the material, there was a tendency to maintain these OD values. ,
Although there was no statistically significant difference (P > 0.05) between the OD of the lining materials at the studied thicknesses, the results indicated that visualization of the materials was possible, but it was not possible to recognize the material that was present. According to the results found, this differentiation was only possible at a thickness of 1.0 mm.
At 0.5 mm, the percentage of radiopacifier was small in comparison to the volume of the material used. The radiographic image of the material was shown to be radiolucent; that is, the amount of material present was not capable of blocking the X-rays along their trajectory, preventing sensitization of the film.  However, at 1.0 mm the amount of radiopacifier was sufficient to allow this sensitizing and there was differentiation in the OD of the materials, due to the presence of different metals in their compositions. , At 1.5 mm, this differentiation in OD no longer existed, because the volume of the radiopacifier agents was no longer relevant and the thickness of the material was predominant for the formation of the radiographic image. 
The other hypothesis tested was that the OD of lining materials differed from those of the dental structures, irrespective of their thickness. Analyses of the results did not allow one to agree with the tested hypothesis, because the radiographic images of the dental structures were confounded with the structures of the materials at some of the thicknesses, as occurred at the thicknesses of 1.5 and 2.0 mm.  Moreover, the dental structures were seen to have a similar OD up to a thickness of 1.5 mm. This was important for differential clinical diagnosis, because it was not possible to distinguish the three structures in the radiographic image. This phenomenon could have occurred because at a thicknesses of up to 1.0 mm, the dental structures were not sufficiently thick to prevent the passage of the X-rays, and formed a radiolucent image on the film. 
The OD value obtained for the enamel and dentin in this study is similar to that found by Williams and Billington,  who have observed a radiopacity value of 2.0 mm of aluminum for enamel and 1.0 mm for dentin. These findings are also in agreement with van Dijken et al., who has shown that the OD of dentin is approximately equivalent to that of aluminum of the same thickness and that enamel is approximately two times more radiopaque than aluminum.
With the 1.5 mm thickness, the results indicated that there was an equivalence between the OD of the dental and material structures, demonstrating that the composition of the lining materials was relevant for the formation of the radiographic image. ,, This fact became clinically relevant, because the use of these materials in the cavity to be restored was indicated for a thickness of 1.5 and 2.0 mm.  In the event that the remaining tooth presented enamel and dentin thicknesses similar to these, there would be no distinction in the radiographic image.
| Conclusions|| |
Analyses of the results allowed the following conclusions to be drawn:
- The thickness of the lining material contributes to its radiopacity. However, for the CH cement, this interference is limited to 2.0 mm.
- It is not possible to differentiate the radiographic images of enamel and dentin at a thickness of up to 1.5 mm.
- The lining materials must not be used at a thickness between 1.5 and 2.0 mm in cases where there are similar thicknesses of dental structures, as it is not possible to differentiate the radiographic images.
| References|| |
|1.||Holland R, de Souza V. Ability of a new calcium hydroxide root canal filling material to induce hard tissue formation. J Endod 1985;11:535-43. [PUBMED] |
|2.||Little PA, Wood DJ, Bubb NL, Maskill SA, Mair LH, Youngson CC. Thermal conductivity through various restorative lining materials. J Dent 2005;33:585-91. [PUBMED] [FULLTEXT] |
|3.||Leonardo MR, da Silva LA, Tanomaru Filho M, Bonifαcio KC, Ito IY. In vitro evaluation of antimicrobial activity of sealers and pastes used in endodontics. J Endod 2000;26:391-4. |
|4.||Estrela C, Estrela CR, Pιcora JD. A study of the time necessary for calcium hydroxide to eliminate microorganisms in infected canals. J Appl Oral Sci 2003;11:133-7. |
|5.||Bullard RH, Leinfelder KF, Russell CM. Effect of coefficient of thermal expansion on microleakage. J Am Dent Assoc 1988;116:871-4. [PUBMED] |
|6.||Kovarik RE, Haubenreich JE, Gore D. Glass ionomer cements: A review of composition, chemistry, and biocompatibility as a dental and medical implant material. J Long Term Eff Med Implants 2005;15:655-71. [PUBMED] [FULLTEXT] |
|7.||Nakajo K, Imazato S, Takahashi Y, Kiba W, Ebisu S, Takahashi N. Fluoride released from glass-ionomer cement is responsible to inhibit the acid production of caries-related oral streptococci. Dent Mater 2009;25:703-8. [PUBMED] [FULLTEXT] |
|8.||Laghios CD, Benson BW, Gutmann JL, Cutler CW. Comparative radiopacity of tetracalcium phosphate and other root-end filling materials. Int Endod J 2000;33:311-5. [PUBMED] [FULLTEXT] |
|9.||Imai Y, Komabayashi T. Properties of a new injectable type of root canal filling resin with adhesiveness to dentin. J Endod 2003;29:20-3. [PUBMED] [FULLTEXT] |
|10.||Tveit AB, Espelid I. Radiographic diagnosis of caries and marginal defects in connection with radiopaque composite fillings. Dent Mater 1986;2:159-62. [PUBMED] |
|11.||Espelid I, Tveit AB, Erickson RL, Keck SC, Glasspoole EA. Radiopacity of restorations and detection of secondary caries. Dent Mater 1991;7:114-7. [PUBMED] [FULLTEXT] |
|12.||Akerboom HB, Kreulen CM, van Amerongen WE, Mol A. Radiopacity of posterior composite resins, composite resin luting cements, and glass ionomer lining cements. J Prosthet Dent 1993;70:351-5. [PUBMED] [FULLTEXT] |
|13.||Hara AT, Serra MC, Haiter-Neto F, Rodrigues AL Jr. Radiopacity of esthetic restorative materials compared with human tooth structure. Am J Dent 2001;14:383-6. [PUBMED] |
|14.||Hara AT, Serra MC, Rodrigues Junior AL. Radiopacity of glass-ionomer/composite resin hybrid materials. Braz Dent J 2001;12:85-9. |
|15.||Turgut MD, Attar N, Onen A. Radiopacity of direct esthetic restorative materials. Oper Dent 2003;28:508-14. [PUBMED] |
|16.||Sidhu SK, Shah PM, Chong BS, Pitt Ford TR. Radiopacity of resin-modified glass-ionomer restorative cements. Quintessence Int 1996;27:639-43. [PUBMED] |
|17.||Anusavice KJ. Chemistry of synthetic resins. Phillip's Science of Dental Materials. In: Anusavice KJ, editor. Philadelphia: Saunders; 2003. p. 211-35. |
|18.||el-Mowafy OM, Benmergui C. Radiopacity of resin-based inlay luting cements. Oper Dent 1994;19:11-5. [PUBMED] |
|19.||Mjor IA. Human coronal dentine: Structure and reactions. Oral Surg Oral Med Oral Pathol 1972;33:810-23. |
|20.||Beyer-Olsen EM, Orstavik D. Radiopacity of root canal sealers. Oral Surg Oral Med Oral Pathol 1981;51:320-8. [PUBMED] |
|21.||Curtis PM Jr, von Fraunhofer JA, Farman AG. The radiographic density of composite restorative resins. Oral Surg Oral Med Oral Pathol 1990;70:226-30. [PUBMED] |
|22.||Gurdal P, Akdeniz BG. Comparison of two methods for radiometric evaluation of resin-based restorative materials. Dentomaxillofac Radiol 1998;27:236-9. |
|23.||Tanomaru-Filho M, Jorge EG, Tanomaru JM, Goncalves M. Evaluation of the radiopacity of calcium hydroxide- and glass-ionomer-based root canal sealers. Int Endod J 2008;41:50-3. |
|24.||Cestari A, Bandeira LC, Calefi PS, Nassar EJ, Ciuffi KJ. Preparation of calcium fluoroaluminosilicate glasses containing sodium and phosphorus by the nonhydrolytic sol-gel method. J Alloys Comp 2009;472:299-306. |
|25.||Darvell BW. Cements and liners. Materials Science for Dentistry. In: Darvell BW, editor. Hong Kong: CRC Press; 2000. p. 181-211. |
|26.||Camilleri J. Characterization and chemical activity of Portland cement and two experimental cements with potential for use in dentistry. Int Endod J 2008;41:791-9. [PUBMED] [FULLTEXT] |
|27.||Manson-Hing LR, Bloxom RM. A stepwedge quality assurance test for machine and processor in dental radiography. J Am Dent Assoc 1985;110:910-3. [PUBMED] |
|28.||Darvell BW. Radiography. Materials Science for Dentistry. In: Darvell BW, editor. Hong Kong: CRC Press; 2000. p. 489-504. |
|29.||Camilleri J, Gandolfi MG. Evaluation of the radiopacity of calcium silicate cements containing different radiopacifiers. Int Endod J 2010;43:21-30. [PUBMED] [FULLTEXT] |
|30.||Watts DC, McCabe JF. Aluminium radiopacity standards for dentistry: An international survey. J Dent 1999;27:73-8. [PUBMED] [FULLTEXT] |
|31.||Guerreiro-Tanomaru JM, Duarte MA, Gonηalves M, Tanomaru-Filho M. Radiopacity evaluation of root canal sealers containing calcium hydroxide and MTA. Braz Oral Res 2009;23:119-23. |
|32.||Gu S, Rasimick BJ, Deutsch AS, Musikant BL. Radiopacity of dental materials using a digital X-ray system. Dent Mater 2006;22:765-70. [PUBMED] [FULLTEXT] |
|33.||Tanomaru-Filho M, da Silva GF, Duarte MA, Gonηalves M, Tanomaru JM. Radiopacity evaluation of root-end filling materials by digitization of images. J Appl Oral Sci 2008;16:376-9. |
|34.||Williams JA, Billington RW. A new technique for measuring the radiopacity of natural tooth substance and restorative materials. J Oral Rehabil 1987;14:267-9. [PUBMED] |
|35.||van Dijken JW, Wing KR, Ruyter IE. An evaluation of the radiopacity of composite restorative materials used in Class I and Class II cavities. Acta Odontol Scand 1989;47:401-7. [PUBMED] |
Lucas FR Garcia
Rua Bernardino de Campos, 30 - apto. 1002, Bairro Higienópolis, 14015-130, Ribeirão Preto, SP
Source of Support: None, Conflict of Interest: None
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5]
[Table 1], [Table 2]
|This article has been cited by|
||Study of the radio-opacity of base and liner dental materials using a digital radiography system
| ||KM Lachowski,SB Botta,CA Lascala,AB Matos,MAP Sobral |
| ||Dentomaxillofacial Radiology. 2013; 42(2): 20120153 |
|[Pubmed] | [DOI]|
| Article Access Statistics|
| Viewed||3106 |
| Printed||149 |
| Emailed||0 |
| PDF Downloaded||279 |
| Comments ||[Add] |
| Cited by others ||1 |